N A N O E X P R E S S
Facile Solution Synthesis of Red
Phosphorus Nanoparticles for Lithium Ion
Fei Wang, Wenwen Zi, Bao Xun Zhao and Hong Bin Du*
Red phosphorus (RP) has attracted extensive attention as an anodic material for lithium-ion batteries (LIBs) due to its high theoretical specific capacity of 2596 mA h g−1 and earth abundance. However, the facile and large-scale preparation of the red phosphorus nanomaterials via a solution synthesis remains a challenge. Herein, we develop a simple and facile solution method to prepare red phosphorus nanoparticles (RP NPs). PCl3readily reacts with HSiCl3in the presence of amines at room temperature to produce amorphous RP NPs with sizes about 100–200 nm in high yields. When used as an anode for rechargeable lithium ion battery, the RP NP electrode exhibits good electrochemical performance with a reversible capacity of 1380 mA h g−1after 100 cycles at a current density of 100 mA g−1, and Coulombic efficiencies reaching almost 100% for each cycle. The study shows that this solution synthesis is a facile and convenient approach for large-scale production of RP NP materials for use in high-performance Li-ion batteries.
Keywords:Red phosphorous, Solution method, Lithium ion battery, Anode material
It has been realized for a long time that fossil fuels are non-renewable, finite, and environmentally harmful. Re-chargeable lithium ion batteries (LIBs) with high energy density and long cycle life have stimulated extensive re-search interest because of their potentials as efficient and cheap energy storage systems [1–3]. The increasing demands for low-cost lithium ion batteries (LIBs) with high energy density and long cycle life call for the devel-opment of novel electrode materials [4–7]. The trad-itional graphite anode, commonly used in lithium ion batteries, is limited with respect to its low capacities (372 mA h g−1) [8,9]. To address this problem or issue, a great deal of efforts have been devoted to explore and develop alternative anode materials with substantially improved capacity and Coulombic efficiencies [10–17]. Among a wide range of high capacity anode materials, phosphorus and its composites show potential applica-tions due to its low cost, abundance and high theoretical specific capacity (≈2600 mA h g−1) [18–22].
Phosphorus has three allotropes, white P, black P, and red P . White P is toxic and chemically unstable, and is not suitable for the application in LIBs. Black P has good thermodynamic stability and conductivity, but the complex preparation process limits its large-scale applica-tions [24–26]. Among these three different allotropes, red P is the most promising candidate  for the next gener-ation high-energy anodic materials because of its stability and abundance. However, red P is plagued by its poor electronic conductivity (10−12S m−1) and drastic volume change (300%) during the lithiation-delithiation process when served as anodes for rechargeable LIBs [28,29].
To circumvent these impediments, red P has been encapsulated in different types of carbon host materials [30–36] to substantially improve the electrochemical per-formance of red P anodes for LIBs. For instance, Li et al. significantly improved both lithium storage and sodium storage performance of red P by confining nanosized amorphous red P into a mesoporous carbon matrix (P@CMK-3) via vaporization-condensation-conversion process . Ruan et al. designed a new strategy to embed red P particles into a cross-link-structural carbon film (P-C film) for use as a flexible binder-free anode in LIBs, in order to improve the electronic conductivity and
State Key Laboratory of Coordination Chemistry, School of Chemistry and Chemical Engineering, Nanjing University, Nanjing 210023, China
duction of PI3 in iodobenzene by ethylene glycol in the
presence of CTAB. The obtained RPNP electrodes exhib-ited a high-specific capacity, long cycling life, and excellent rate capability as anodes for LIBs . Moreover, Zhou et al. reported a wet solvothermal method to synthesize hol-low red-phosphorous nanospheres with porous shells. The obtained hollow P nanosphere electrodes demonstrated high capacities and excellent long cycling performance due to the merits of the porous and hollow structures . Even though several literatures have reported the methods to the large-scale synthesis of red phosphorus, developing a high-yield and low-cost facile method to pre-pare the red phosphorus is still highly desirable. Particu-larly, the preparation of the red phosphorus nanomaterial via a solution synthesis remains a challenge.
Herein, we report a facile, rapid, and novel solution-based approach to synthesize RP NPs, employing room-temperature reaction of PCl3with HSiCl3in CH2Cl2
in the presence of amines. This new solution provides a cost-effective approach for massive production of red phosphorus nanoparticles for use in lithium ion batteries.
Trichlorosilane (HSiCl3) was purchased from TCI.
n-Tripropylamine (Pr3N) was obtained from Aladdin.
Phos-phorus trichloride (PCl3) was purchased from Sinopharm
Chemical Reagent Co. Ltd. Dichloromethane (CH2Cl2) was
dried over CaH2 before use. All other chemical reagents
were used as received without further purification.
Synthesis of Red Phosphorus Nanoparticles
In a typical preparation, 0.55 mL of Pr3N and 0.5 mL of
HSiCl3 were added into 20 mL of anhydrous CH2Cl2.
The formed colorless solution was magnetically stirred overnight at room temperature, during which the color turned into light yellow. And then 0.5 mL of PCl3were
added to the solution. Red phosphorus nanoparticles (RP NPs) were obtained in several seconds. The prod-ucts were centrifuged, separated, and washed with an-hydrous CH2Cl2, 1 M HF and distilled water to remove
unreacted PCl3and silica.
drying at 80 °C for 12 h in vacuum, the foil was cut into disks of 14 mm in diameter. The total mass loading of ac-tive materials on the electrode was ~ 0.5 mg cm−2. The electrolyte was 1.0 M LiPF6in a mixture of 1:1 (v/v)
ethyl-ene carbonate/diethyl carbonate (Shenzhen Kejingstar Technology Ltd., China). The charge-discharge profiles of the half-cells were recorded using a Neware battery testing device (Shenzhen, China) at a constant current mode.
Powder X-ray diffraction (PXRD) was carried on a Bruker D8 X-ray diffractometer with a Cu Kα radiation (λ= 1.5418 Å). Scanning electron microscopy (SEM) images and energy dispersive spectroscopy (EDS) spectra (silicon wafers as the substrate) were obtained on a Hitachi field-emission scanning electron microscope (S-4800). Transmission electron microscopy (TEM) and high-reso-lution (HR) TEM were carried out with a JEM-2100 equipment (Japan). N2 adsorption isotherms were
col-lected at 77 K (Micromeritics ASAP 2020 analyzer) after vacuum degassing of the sample at 100 °C for 10 h. Raman spectroscopy (LabRAM Aramis, Horiba, equipped with 633 nm laser) was used to investigate the structure of RP NPs. X ray photoelectron spectroscopy (XPS) measure-ments were recorded with a PHI 5000 VersaProbe. Thermo gravimetric (TG) analyses were conducted on a simultaneous STA449F3 (Netzche) thermal analyzer under flowing N2. The I-V curves of RP NPs were
mea-sured using cryogenic probe station Biologic VMP3 in-strument (CRX-4K, Lake Shore, USA). Cyclic voltam metry (CV) tests were performed on a CHI650d electro-chemical station (Shanghai Chenhua Instruments Inc., China).
Results and Discussion
Synthesis and Characterization of RPNPs
The red phosphorus nanoparticles (denoted as RP NPs) were synthesized via a facile solution method, which is depicted in Scheme 1. We found that phosphorus tri-chloride (PCl3) readily reacted with premixed HSiCl3
and tripropylamine (Pr3N) in CH2Cl2 at room tempera
mixing a solution of HSiCl3–Pr3N–CH2Cl2with PCl3,
in-dicating the formation of RP NPs (Additional file1: Figure S1). We postulated that PCl3were reduced by subvalent
oligosilane chlorides to form the phosphorus nanoparti-cles. The oligosilane chlorides were formed by the reaction of HSiCl3with tripropylamine (Pr3N) in CH2Cl2as results
of disproportionation reaction of HSiCl3 in the presence
of amine catalysts [45–47]. It is noted that the preformed oligosilane intermediates were essential for the occurrence of the reaction. Without amines (Pr3N), the reaction of
HSiCl3 with PCl3 could not take place at room
temperature. Similarly, the Pr3N could not react with PCl3
to produce RP NPs at room temperature. The yield of RP NPs, based on the amount of P atoms in PCl3, was
ap-proximately 38%, which is much higher than the reported literature . Furthermore, this solution-phase approach utilizes relatively low cost PCl3instead of PI3in
iodoben-zene, which could be more economically and easily scaled up to obtain large amounts of RP NPs. The color of the RPNPs was light orange, differing from the deep red color of commercial RP (Additional file1: Figure S2).
PXRD analysis showed that the product was red phos-phorus. As shown in Fig. 1a, the three broadened dif-fraction peaks at 13–16°, 25–38°, and 47–65°, consistent
with the XRD pattern of commercial RP reported in the literature [21,36]. SEM images show that the majority of RP NPs synthesized exhibited irregular-spherical shape with sizes about 100–200 nm in diameter. The corre-sponding SAED pattern of RP NPs (inset image of Fig.2b) revealed that RP NPs were amorphous structure. Raman spectra of RP NPs presented three puckered peaks between 300 and 500 cm−1, which is consistent with the Raman spectrum of commercial RP reported in the literature . The three peaks can be well assigned to the bond bending modes (B1 fundamental mode), bond bending vibrations (A1 symmetric stretch motion), and stretching vibrations (E1 degenerate mode) of amorphous red P (Fig.1b). The thermal gravimetric ana-lysis (TGA) of RPNPs in Fig. 3a shows a sharp weight loss between 380 and 430 °C under a nitrogen atmos-phere owing to the sublimation, whereas commercial RP shows a sharp weight loss between 450 and 500 °C. The observed depression of sublimation temperature of RP NPs may result from high surface-to-volume ratios of nanoparticles [43,48]. To quantitatively obtain the infor-mation of surface area, N2 sorption measurements
(Fig. 3b) were conducted. The results revealed the Bru-nauer–Emmett–Teller (BET) surface area of RP NPs was
Scheme 1Schematic illustration of the synthesis process of RP NPs
about 37 m2g−1, which is much larger than that of the commercial RP.
In order to further characterize the structures, compo-sitions, and chemical states of the prepared RP NPs, energy-dispersive X-ray spectroscopy (EDS) and X-ray photoelectron spectroscopy (XPS) measurements were carried out (Fig.4). The EDS spectra shows that RP NPs are almost completely composed of elemental phos-phorus. XPS survey spectrum (Fig.4b) further confirms that P is the dominant element. The main peak in P 2p spectrum of XPS could be deconvoluted into two peaks at 129.74 and 130.74 eV, which correspond to the 2p3/2
and 2p1/2 of P in P–P bond, respectively, according to
the previous literature [49, 50]. Moreover, a weak peak at 133.50 eV could be assigned to the P–O bond which was possibly formed through surface oxidation during air exposure. Therefore, the above results indicate the prepared nanoparticles are amorphous red P. In addition, the current-voltage (I-V) curves of RP NPs have been measured, as shown in Additional file 1: Figure S3. The conductivity of the RPNPs is about 1.7 × 10−7 S m−1 (0–2 V), which is 105 times higher than commercial RP (10−12S m−1).
The electrochemical performance of the RP NPs as anode materials in LIBs was tested in CR2032 coin cells using a lithium metal foil as the counter electrode within the operating voltages of 0.01 to 2.5 V. Figure5adepicts
typical CV curves of the RP NPs at a scanning rate of 0.1 mV s−1. There is a broad peak in the first lithiation cycle, which is ascribed to the activation process of inserting Li ions into phosphorus. A couple of redox peaks located at 0.5–0.75 V and 1.0–1.25 V are attrib-uted to the lithiation of P and the delithiation of P–Li al-loys [32,51,52] respectively. The deviation between the first and the subsequent cathodic curves implies irre-versible capacity loss, which could be ascribed to the for-mation of the solid electrolyte interface (SEI) as well as to the occurrence of side reactions on the electrode sur-faces, such as side reactions of defect sites, surface oxy-gen, and water impurities [36, 37, 53], a commonly observed behavior for LIB anodes. Figure 5b shows the typical discharge-charge voltage profiles of the RP NPs electrode for the first 3 cycles at a current density of 0.1 A g−1. The apparent short discharge and charge volt-age plateaus at around 0.7 V and 1.1 V are due to the lithiation and de-lithiation of RP NPs components, re-spectively, which agree well with the CV results. The electrode delivered a specific discharge and charge cap-acities of 2818 and 1641 mA h g−1, respectively, for the first cycle, giving a first Coulombic efficiency of 58.2%. The decreased charge capacity could be attributed to the irreversible formation of the SEI membrane. It is noted that the Coulombic efficiency of RP NPs then quickly increased to 100% after the second cycle. The RP NPs
Fig. 2Morphology of RP NPs.aSEM images of RP NPs.bTEM images of RP NPs. The inset image is the SAED pattern
Fig. 4aEDS spectra of RP NPs.bP 2p XPS spectrum of RP NPs
spectively. RPNPs delivered the specific charge capacities of 1801, 1430, 1245, 1227, 1184, and 871 mA h g−1at the rates of 0.1, 0.2, 0.3, 0.5, and 1 A g−1, respectively. The electrode showed good rate reversibility, with the specific discharge capacity recovered to the initial value when the current density returned to 0.1 A g−1after cycling at high current densities. The RP NPs finally maintained a high reversible discharge capacity of 1380 mA h g−1, i.e., the re-tention of 89.1%, after 100 cycles with Coulombic efficien-cies close to 100% throughout the measurements. Compared to commercial RP (Fig. 5e), RP NPs showed much improved long-term cycling stability.
In summary, we developed a new facile solution-phase ap-proach to synthesis red phosphorus nanoparticles through the reaction of PCl3and HSiCl3in the presence of amines
under the ambient environment. The RP NPs exhibited much better electrochemical performance with high re-versible capacity and long-term cycling stability than com-mercial RP when served as anodes for rechargeable lithium ion battery. The RP NPs electrodes maintained a high reversible discharge capacity of 1380 mA h g−1 (retention of 89.1%) after 100 cycles, with a Coulombic ef-ficiency close to 100% for each cycle. This simple prepar-ation method paves the way for cost-effective production of RP NPs as high-performance anodes for lithium-ion battery industry.
Additional file 1:Figure S1.The reaction process of RPNPs via the solution synthesis.Figure S2.Optical images of RPNPs and commercial RP powders.Figure S3.I-V curves of RPNPs. Figure S4. SEM images of commercial RP. (DOCX 631 kb)
CH2Cl2:Dichloromethane; CV: Cyclic voltammetry; EDS: Energy dispersive
spectroscopy; HSiCl3: Trichlorosilane; PCl3: Phosphorus trichloride; Pr3N:
n-Tripropylamine; PXRD: Powder X-ray diffraction; RP NPs: Red phosphorus nanoparticles; SEM: Scanning electron microscopy; TEM: Transmission electron microscopy; TG: Thermo gravimetric; XPS: X-ray photoelectron spectroscopy
Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Received: 28 August 2018 Accepted: 23 October 2018
1. Etacheri V, Marom R, Elazari R, Salitra G, Aurbach D (2011) Challenges in the development of advanced Li-ion batteries: a review. Energy Environ Sci 4(9): 3243–3262
2. Goriparti S, Miele E, De Angelis F, Di Fabrizio E, Proietti Zaccaria R, Capiglia C (2011) Review on recent progress of nanostructured anode materials for Li-ion batteries. J Power Sources 257:421–443
3. Ellis BL, Lee KT, Nazar LF (2010) Positive electrode materials for ion and Li-batteries. Chem Mater 2(3):691–714
4. Tarascon JM, Armand M (2001) Issues and challenges facing rechargeable lithium batteries. Nature 414:359–367
5. Bruce PG, Scrosati B, Tarascon JM (2008) Nanomaterials for rechargeable lithium batteries. Angew Chem Int Ed 47(16):2930–2946
6. Feng K, Li M, Liu W, Kashkooli AG, Xiao X, Cai M, Chen Z (2018) Silicon-based anodes for lithium-ion batteries: from fundamentals to practical applications. Small 14(1):1702737–1702770
7. Gonzalez AF, Yang NH, Liu RS (2017) Silicon anode design for lithium-ion batteries: progress and perspectives. J Phys Chem C 121(50):27775–27787 8. Kaskhedikar NA, Maier J (2009) Lithium storage in carbon nanostructures.
Adv Mater 21(25–26):2664–2680
9. Mao Y, Duan H, Xu B, Zhang L, Hu Y, Zhao C, Wang Z, Chen L, Yang Y (2012) Lithium storage in nitrogen-rich mesoporous carbon materials. Energy Environ Sci 5(7):7950–7955
10. Kumai Y, Kadoura H, Sudo E, Iwaki M, Okamoto H, Sugiyama Y, Nakano H (2011) Si–C composite anode of layered polysilane (Si6H6) and sucrose for
lithium ion rechargeable batteries. J Mater Chem 21(32):11941–11946 11. Ge M, Rong J, Fang X, Zhang A, Lu Y, Zhou C (2013) Scalable preparation of
porous silicon nanoparticles and their application for lithium-ion battery anodes. Nano Res 6(3):174–181
12. Jia H, Gao P, Yang J, Wang J, Nuli Y, Yang Z (2011) Novel three-dimensional mesoporous silicon for high power lithium-ion battery anode material. Adv Energy Mater 1(6):1036–1039
13. Luo J, Liu J, Zeng Z, Ng CF, Ma L, Zhang H, Lin J, Shen Z, Fan HJ (2013) Three-dimensional graphene foam supported Fe3O4lithium battery anodes
with long cycle life and high rate capability. Nano Lett 13(12):6136–6143 14. Jing M, Zhou M, Li G, Chen Z, Xu W, Chen X, Hou Z (2017)
Graphene-embedded Co3O4rose-spheres for enhanced performance in lithium ion
batteries. ACS Appl Mater Interfaces 9(11):9662–9668
15. Lu B, Ma B, Deng X, Li W, Wu Z, Shu H, Wang X (2017) Cornlike ordered mesoporous silicon particles modified by nitrogen-doped carbon layer for the application of Li-Ion battery. ACS Appl Mater Interfaces 9(38):32829–32839 16. Lv G, Zhu B, Li X, Chen C, Li J, Jin Y, Hu X, Zhu J (2017) Simultaneous
perforation and doping of Si nanoparticles for lithium-ion battery anode. ACS Appl Mater Interfaces 9(51):44452–44457
17. Ma Q, Wang W, Zeng P, Fang Z (2017) Amorphous Ge/C composite sponges: synthesis and application in a high-rate anode for lithium ion batteries. Langmuir 33(9):2141–2147
black phosphorus nanoparticle-graphite composite battery anodes. Nano Lett 14(8):4573–4580
19. Qian J, Wu X, Cao Y, Ai X, Yang H (2013) High capacity and rate capability of amorphous phosphorus for sodium ion batteries. Angew Chem Int Ed 125(17):4731–4734
20. Huang S, Cheong LZ, Wang D, Shen C (2017) Nanostructured phosphorus doped silicon/graphite composite as anode for high-performance lithium-ion batteries. ACS Appl Mater Interfaces 9(28):23672–23678
21. Kim Y, Park Y, Choi A, Choi NS, Kim J, Lee J, Ryu JH, Oh SM, Lee KT (2013) An amorphous red phosphorus/carbon composite as a promising anode material for sodium ion batteries. Adv Mater 25(22):3045–3049 22. Gao H, Zhou T, Zheng Y, Liu Y, Chen J, Liu H, Guo Z (2016) Integrated
carbon/red phosphorus/graphene aerogel 3D architecture via advanced vapor-redistribution for high-energy sodium-ion batteries. Adv Energy Mater 6(21):1601037–1601044
23. Park CM, Sohn HJ (2007) Black phosphorus and its composite for lithium rechargeable batteries. Adv Mater 19(18):2465–2468
24. Zhang Y, Zheng Y, Rui K, Hng HH, Hippalgaonkar K, Xu J, Sun W, Zhu J, Yan Q, Huang W (2017) 2D black phosphorus for energy storage and thermoelectric applications. Small 13:1700661–1700681
25. Li QF, Duan CG, Wan XG, Kuo JL (2015) Theoretical prediction of anode materials in li-ion batteries on layered black and blue phosphorus. J Phys Chem C 119(16):8662–8670
26. Liu H, Du Y, Deng Y, Ye D (2015) Semiconducting black phosphorus: synthesis, transport properties and electronic applications. Chem Soc Rev 44:2732–2743
27. Zhou J, Jiang Z, Niu S, Zhu S, Zhou J, Zhu Y, Liang J, Han D, Xu K, Zhu L, Liu X, Wang G, Qian Y (2018) Self-standing hierarchical P/CNTs@rGO with unprecedented capacity and stability for lithium and sodium storage. Chem 4(2):372–385
28. Zaug JM, Soper AK, Clark SM (2008) Pressure-dependent structures of amorphous red phosphorus and the origin of the first sharp diffraction peaks. Nature Mater 7(11):890–899
29. Yabuuchi N, Matsuura Y, Ishikawa T, Kuze S, Son JY, Cui YT, Oji H, Komaba S (2014) Phosphorus electrodes in sodium cells: small volume expansion by sodiation and the surface-stabilization mechanism in aprotic solvent. Chem Electro Chem 1(3):580–589
30. Zhu Y, Wen Y, Fan X, Gao T, Han F, Luo C, Liou SC, Wang C (2015) Red phosphorus–single-walled carbon nanotube composite as a superior anode for sodium ion batteries. ACS Nano 9(3):3254–3264
31. Sun J, Lee HW, Pasta M, Sun Y, Liu W, Li Y, Lee HR, Liu N, Cui Y (2016) Carbothermic reduction synthesis of red phosphorus-filled 3D carbon material as a high-capacity anode for sodium ion batteries. Energy Storage Mater 4:130–136 32. Yuan D, Cheng J, Qu G, Li X, Ni W, Wang B, Liu H (2016) Amorphous red
phosphorous embedded in carbon nanotubes scaffold as promising anode materials for lithium-ion batteries. J Power Sources 301:131–137
33. Li W, Hu S, Luo X, Li Z, Sun X, Li M, Liu F, Yu Y (2017) Confined amorphous red phosphorus in MOF-derived N-doped microporous carbon as a superior anode for sodium-ion battery. Adv Mater 29(16):1605820–1605828 34. Song J, Yu Z, Gordin ML, Li X, Peng H, Wang D (2015) Advanced sodium ion
battery anode constructed via chemical bonding between phosphorus, carbon nanotube, and cross-linked polymer binder. ACS Nano 9(12):11933–11941 35. Yu Z, Song J, Gordin ML, Yi R, Tang D, Wang D (2015) Phosphorus-graphene
nanosheet hybrids as lithium-ion anode with exceptional high-temperature cycling stability. Adv Sci 2(1–2):1400020–1400027
36. Li WJ, Chou SL, Wang JZ, Liu HK, Dou SX (2013) Simply mixed commercial red phosphorus and carbon nanotube composite with exceptionally reversible sodium-ion storage. Nano Lett 13(11):5480–5484
37. Li W, Yang Z, Li M, Jiang Y, Wei X, Zhong X, Gu L, Yu Y (2016) Amorphous red phosphorus embedded in highly ordered mesoporous carbon with superior lithium and sodium storage capacity. Nano Lett 16(3):1546–1553 38. Ruan J, Yuan T, Pang Y, Xu X, Yang J, Hu W, Zhong C, Ma ZF, Bi X, Zheng S
(2017) Red phosphorus-embedded cross-link-structural carbon films as flexible anodes for highly reversible li-ion storage. ACS Appl Mater Interfaces 9(41):36261–36268
39. Marino C, Debenedetti A, Fraisse B, Favier F, Monconduit L (2011) Activated-phosphorus as new electrode material for li-ion batteries. Electrochem Commun 13(4):346–349
40. Wang L, He X, Li J, Sun W, Gao J, Guo J, Jiang C (2012) Nano-structured phosphorus composite as high-capacity anode materials for lithium batteries. Angew Chem Int Ed 51(36):9034–9037
41. Zhang Y, Rui X, Tang Y, Liu Y, Wei J, Chen S, Leow WR, Li W, Liu Y, Deng J, Ma B, Yan Q, Chen X (2016) Wet-chemical processing of phosphorus composite nanosheets for high-rate and high-capacity lithium-ion batteries. Adv Energy Mater 6(10):1502409–1502418
42. Winchester RA, Whitby M, Shaffer MS (2009) Synthesis of pure phosphorus nanostructures. Angew Chem Int Ed 48(20):3616–3621
43. Chang WC, Tseng KW, Tuan HY (2017) Solution synthesis of iodine-doped red phosphorus nanoparticles for lithium-ion battery anodes. Nano Lett 17(2):1240–1247
44. Zhou J, Liu X, Cai W, Zhu Y, Liang J, Zhang K, Lan Y, Jiang Z, Wang G, Qian Y (2017) Wet-chemical synthesis of hollow red-phosphorus nanospheres with porous shells as anodes for high-performance lithium-ion and sodium-ion batteries. Adv Mater 29(29):1700214–1700221
45. Tillmann J, Wender JH, Bahr U, Bolte M, Lerner HW, Holthausen MC, Wagner M (2015) One-step synthesis of a silafullerane with an endohedral chloride ion. Angew Chem Int Ed 54(18):5429–5433
46. Choi SB, Kim BK, Boudjouk P, Grier DD (2001) Amine-promoted disproportionation and redistribution of trichlorosilane: formation of tetradecachlorocyclohexasilane dianion. J Am Chem Soc 123(33):8117–8118 47. Tillmann J, Meyer L, Schweizer JI, Bolte M, Lerner HW, Wagner M, Holthausen
MC (2014) Chloride-induced aufbau of perchlorinated cyclohexasilanes from Si2Cl6: a mechanistic scenario. Chem Eur J 20(30):9234–9239
48. Qi WH, Wang MP (2004) Size and shape dependent melting temperature of metallic nanoparticles. Mater Chem Phys 88(2–3):280–284
49. Li WJ, Chou SL, Wang JZ, Liu HK, Dou SX (2016) Significant enhancement of the cycling performance and rate capability of the P/C composite via chemical bonding (P-C). J Mater Chem A 4(2):505–511
50. Song J, Yu Z, Gordin ML, Hu S, Yi R, Tang D, Walter T, Regula M, Choi D, Li X, Manivannan A, Wang D (2014) Chemically bonded phosphorus/graphene hybrid as a high performance anode for sodium-ion batteries. Nano Lett 14(11):6329–6335
51. Qian J, Qiao D, Ai X, Cao Y, Yang H (2012) Reversible 3-li storage reactions of amorphous phosphorus as high capacity and cycling-stable anodes for li-ion batteries. Chem Commun 48(71):8931–8933
52. Yuan T, Ruan J, Peng C, Sun H, Pang Y, Yang J, Ma ZF, Zheng S (2018) 3D red phosphorus/sheared CNT sponge for high performance lithium-ion battery anodes. Energy Storage Mater 13:267–273
53. Wang B, Li X, Zhang X, Luo B, Jin M, Liang M, Dayeh SA, Picraux ST, Zhi L (2013) Adaptable silicon–carbon nanocables sandwiched between reduced graphene oxide sheets as lithium ion battery anodes. ACS Nano 7(2):1437–1445 54. Sun L, Wang F, Su T, Du H (2017) Room-temperature solution synthesis of